arXiv:1704.06402v1 [cond-mat.mtrl-sci] 21 Apr 2017
Time- and spatially-resolved magnetization dynamics driven by spin-orbit torques M. Baumgartner,1 K. Garello,1,2 J. Mendil,1 C. O. Avci,1 E. Grimaldi,1 C. Murer,1 J. Feng,1 M. Gabureac,1 C. Stamm,1 Y. Acremann,3 S. Finizio,4 S. Wintz,4 J. Raabe,4 P. Gambardella1 1
Department of Materials, ETH Z¨ urich, 8093 Z¨ urich, Switzerland, 2
IMEC, Kapeldreef 75, 3001 Leuven, Belgium,
Laboratory for Solid State Physics, ETH Z¨ urich, 8093 Z¨ urich, Switzerland, 4
Paul Scherrer Institute, 5232 Villigen PSI, Switzerland
Abstract Current-induced spin-orbit torques (SOTs) represent one of the most effective ways to manipulate the magnetization in spintronic devices. The orthogonal torquemagnetization geometry, the strong damping, and the large domain wall velocities inherent to materials with strong spin-orbit coupling make SOTs especially appealing for fast switching applications in nonvolatile memory and logic units. So far, however, the timescale and evolution of the magnetization during the switching process have remained undetected. Here, we report the direct observation of SOTdriven magnetization dynamics in Pt/Co/AlOx dots during current pulse injection. Time-resolved x-ray images with 25 nm spatial and 100 ps temporal resolution reveal that switching is achieved within the duration of a sub-ns current pulse by the fast nucleation of an inverted domain at the edge of the dot and propagation of a tilted domain wall across the dot. The nucleation point is deterministic and alternates between the four dot quadrants depending on the sign of the magnetization, current, and external field. Our measurements reveal how the magnetic symmetry is broken by the concerted action of both damping-like and field-like SOT and show that reproducible switching events can be obtained for over 1012 reversal cycles.
Controlling the magnetic state of ultrathin heterostructures using electric currents is key to developing nonvolatile memory devices with minimal static and dynamic power consumption 1 . A promising approach for magnetic switching is based on injecting an in-plane current into a ferromagnet/heavy metal bilayer, where the spin-orbit torques (SOTs) 2,3 resulting from the spin Hall effect and interface charge-spin conversion 4–8 provide an efficient mechanism to reverse the magnetization 1,9,10,12–15 and manipulate domain walls (DWs) 16–19 . SOT switching schemes can be easily integrated into three-terminal magnetic tunnel junctions having either in-plane 10 or out-of-plane 20 magnetization. Although the threeterminal geometry is more demanding in terms of size, it offers desirable features compared to the two-terminal spin-transfer torque (STT) approach presently used in magnetic random access memories (MRAM) 21 . One such feature is the separation of the read and write current paths in the tunnel junction, which avoids electrical stress of the oxide barrier during writing and allows for independent optimization of the tunneling magnetoresistance during reading. The other crucial feature is the switching speed, which is expected to be extremely fast because the spin accumulation inducing the SOTs is orthogonal to the quiescent magnetization, leading to a negligible incubation delay. Such a delay is a major issue for STT devices, since thermal fluctuations result in a switching time distribution that is several ns wide 22,23 . Furthermore, the SOT-induced magnetization dynamics is governed by strong damping in the monodomain regime 24,25 and fast domain wall motion in the multidomain regime 16–18 , both favoring rapid reversal of the magnetization. Recent investigations of SOTs in ferromagnet/heavy metal layers showed that reliable switching can be achieved by the injection of current pulses as short as 200 ps in Pt/Co and Ta/CoFeB structures 1,26,27 . However, these experiments only measured the switching probability as a function of pulse amplitude and duration, while the mechanism and the timescale of magnetization reversal remain unknown. Microscopy studies performed using the magneto-optic Kerr effect have extensively probed SOT-induced DW displacements 14–19,28 , revealing the role played by the Dzyaloshinskii-Moriya interaction (DMI) in stabilizing chiral DW structures that have very high mobility 17,18,29–33 . Such investigations have a spatial resolution of the order of 1 µm, but only probed the static magnetization after current injection, similar to the pulsed switching experiments 1,26,27 . In parallel to this activity, several theoretical models have been proposed in order to elucidate the SOT-induced dynamics. The most straightforward approach is based on the macrospin approximation 24,25,34,35 , which applies in the limit of small magnets and coherent rotation of the magnetization. Under these assumptions, the damping-like (DL) torque TDL ∝ M × (y × M) induces the rotation of the magnetization (M) while the field-like (FL) torque TF L ∝ M×y favors precessional motion of the magnetization about the y-axis, orthogonal to the current. Such a model is often used to relate the critical 1
switching current to the SOT amplitude in practical devices 12,26 , even though the reversal mode is still a matter of debate. A second model is based on the random nucleation and isotropic expansion of magnetic bubbles, induced by a thermally-assisted DW depinning process and the DL component of the SOT 36 . Finally, micromagnetic models have been proposed, in which domain nucleation is either random and thermally-assisted 32,37 or determined by the competition between external field and DMI at the sample edge followed by DW propagation across the magnetic layer 5,39 . In such schemes, which apply to perpendicularly magnetized layers, the DL torque acts as a z-axis field B DL ∝ Mx on the internal DW magnetization, favoring the expansion of a domain on the side where |Mx | is larger (for example at an up-down DW of the type ↑←↓ rather than at the opposite down-up DW ↓→↑). Despite these considerable efforts, a number of issues remain outstanding. The most prominent concern the actual timescale and physical processes that govern the magnetization dynamics during and after current injection, the initial and intermediate magnetic configuration preceding switching, as well as the role played by the DL and FL components of the torque and the DMI. Here, we report the direct observation of the dynamics excited by SOTs during the switching process by performing current-pump and x-ray probe experiments in the time domain using a scanning transmission x-ray microscope (STXM) 40 . Our measurements reveal the evolution of the nanoscale magnetization from the initial domain nucleation stage to full or partial switching, depending on the duration and amplitude of the current pulses. These results determine the actual speed of the switching process and show how the reversal path is unique to SOTs and predetermined by the interplay of the current-induced torques, DMI, and external magnetic field. We find four different configurations of the nucleation point and fast direction of DW propagation, corresponding to the four possible combinations of current and field polarization. The STXM data, combined with micromagnetic simulations and all-electrical measurements of the switching probability, provide a consistent picture of the switching process and evidence how the FL torque influences the reversal path together with the DL torque and DMI. Finally, we show that switching is robust with respect to repeated cycling events as well as to the presence of defects in the sample magnetic structure, which is very promising for the application of SOTs in MRAM devices. Time-resolved switching We studied circular-shaped Co dots with perpendicular magnetization that are 1 nm thick and 500 nm in diameter, capped by 2 nm AlOx and deposited on a 750 nm wide, 5 nm thick Pt current line. The samples were fabricated using electron-beam lithography on transparent Si3 N4 membranes suitable for x-ray transmission and contacted by Au leads, as illustrated in Fig. 1c. Replicas of the dots with four electrical contacts were fabricated on Si3 N4 membranes for all-electrical pulsed switching 2
Figure 1: Schematic of the experimental setup and sample structure. a, A circularly polarized x-ray beam is focused to a 25 nm spot by a zone plate and an order selecting aperture (OSA). The transmission of the x-rays through the sample is monitored by an avalanche photodiode as the sample stage is scanned in steps of 12-25 nm across the x-ray focus. b, Representative STXM image of a Co dot and Pt line showing topographic and elemental contrast at a photon energy of 779 eV. The darker regions indicate the position of the Au contact pads and of the Co dot, which absorb x-rays more strongly than the bare Pt and Si3 N4 regions. c, Magnetic contrast due to the XMCD effect: magnetization pointing parallel or anti-parallel to the x-ray helicity results in different absorption intensity. Black (white) contrast indicates Mz > 0 (Mz < 0). d, Scheme of the pump current circuit. together with Hall bar structures for SOT measurements (see Supplementary Information). Figure 1b shows a static image of the Co dot and Pt line obtained by scanning the sample under the focused x-ray beam. Time-resolved images of the Co magnetization were recorded stroboscopically by probing the transmitted x-ray intensity at the Co L3 absorption edge, where x-ray magnetic circular dichroism (XMCD) provides contrast to the out-of-plane component of the magnetization (Mz ), as shown in Fig. 1c. The pump current consists of a sequence of negative (set) and positive (reset) pulses of variable length and amplitude with a period of 102.1 ns, corresponding to a switching rate of about 20 MHz. An in-plane magnetic field Bx was applied along the current direction in 3
Figure 2: Time-resolved magnetization switching. XMCD time traces showing reversal of the magnetization during the injection of 2 ns long current pulses of opposite polarity at a, Bx = 94 mT and b, Bx = −124 mT. The sign of the XMCD signal is positive for Mz < 0 and negative for Mz > 0. c, Asymmetric set-reset sequence in which the first and second pulses are 2 ns and 0.8 ns long, respectively. d, Fast toggle sequence consisting of two 1 ns long current pulses of opposite polarity separated by 1 ns with inplane field Bx = 92 mT. Up = 1 V corresponds to a current density jp = 8.4 · 107 A/cm2 in the Pt line. order to uniquely define the switching polarity 9 . Figure 2a shows the XMCD time trace obtained by integrating the transmitted x-ray intensity over the entire area of the Co dot during the current pulse sequence, which was separately recorded by a fast oscilloscope in parallel with the sample. The pulses in this sequence are 2 ns long, with a rise time of about 150 ps, and have a separation of 50 ns. The XMCD time trace shows that the magnetization switches from down to up during the first (negative) pulse and from up to down during the second (positive) pulse. The timescale over which Mz changes between two states with opposite saturation magnetization coincides with the duration of the current pulses, indicating that the magnetization is fully reversed within the pulse interval, with no significant delay or after-pulse relaxation.
The response of the magnetization to the current pulses inverts upon changing the sign of Bx , as shown in Fig. 2b, consistently with previous reports of SOT-induced switching of perpendicularly magnetized layers 1,9,10,12–14,17 . Further, we find that the switching speed increases by increasing the current amplitude, allowing for full magnetization reversal within a sub-ns current pulse (Fig. 2c). This speed, and the absence of after-effects, enable the realization of very fast magnetic-writing cycles. One such cycle is shown in Fig. 2d, where we toggle the magnetization between up and down states using a 1 ns on | 1 ns off | 1 ns on pulse sequence. Remarkably, our samples survive uninterrupted pulse sequences for hours without appreciable magnetic or electrical degradation. We tested more than 1012 consecutive and successful switching events, at current densities of the order of 2 − 4 · 108 A/cm2 . Thus, the combination of speed and endurance revealed by our measurements is extremely promising for the operation of SOT-based MRAM and logic devices. Spatial evolution of the magnetization during current injection We next focus on the transient magnetic configurations and the mechanisms leading to magnetization reversal. Figure 3a shows four series of consecutive images recorded at time intervals of 100 ps during the switching process, corresponding to the four possible combinations of current and field polarity. The magnetization reverses by domain nucleation and propagation in all cases, with no appreciable incubation delay. Although the stroboscopic character of our measurements does not allow us to investigate stochastic effects, the observation of a clear DW front moving from a fixed nucleation point on one side of the sample to the opposite side, as shown by the red dots and green arrows in Fig. 3a, indicates that the reversal process is reproducible and deterministic. Furthermore, as we argue in the following, such a reversal scheme is unique to SOTs. Our data show that domain nucleation takes place at the edge of the sample where the DMI and Bx concur to tilt the magnetization towards the current direction, thereby confirming the prediction of recent micromagnetic models 5,39 . However, the concerted action of B DL , DMI, and Bx only leads to a left/right asymmetry, similar to the asymmetric nucleation induced by a perpendicular magnetic field 41 , whereas we observe that the domain nucleation site alternates between the four quadrants shown in Fig. 3b, with an additional top/bottom asymmetry. Edge nucleation To explain this additional asymmetry, we have to analyze the effects of the static and dynamic fields in more detail. Pt/Co/AlOx layers have positive DMI, which stabilizes left-handed N´eel-DW 42 and induces canting of the magnetization at the edge of the dot. In the absence of current and external field, the magnetic moments are symmetrically canted inwards (outwards) of the dot for Mz > 0 (Mz < 0), as illustrated 5
Figure 3: Evolution of the magnetization during the switching process. a, Images taken at intervals of 100 ps during the injection of 2 ns long current pulses. Rows (I,II) and (III,IV) correspond to the time traces shown in Fig. 2a and b, respectively. The red dots indicate the DW nucleation point and the green arrows its propagation direction. The images are low-pass filtered for better contrast (see the Supplementary Information for the raw data and movies). b, Schematic representation of the observed DW nucleation and propagation geometry. Illustration of the DW nucleation process corresponding to case (II): c, Canting of the magnetization at the dot edges induced by the DMI. d, Breaking of the canting symmetry induced by Bx . e, Action of BθDL and BθF L . in Fig. 3c. Upon applying a static field Bx , the canting angle increases on one side, while it decreases on the other (Fig. 3d), favoring domain nucleation on the side where the canting is larger. The injection of a positive current pulse generates an effective DL field with a polar component BθDL that points toward the current direction (purple arrow in Fig. 3e). For a positive Bx , BθDL thus leads to left nucleation if Mz > 0 and no nucleation if Mz < 0. A similar reasoning is valid for all four combinations of field and current polarity leading to magnetization switching, which explains the left/right asymmetry observed in our data. The top/bottom asymmetry, however, can be explained only if an additional torque plays a significant role in the nucleation process. In the following, we argue that the FL torque, combined with the DMI-induced canting at the sample edges, accounts for such an asymmetry. Because the corresponding effective field B F L points 6
Figure 4: Effect of an external field balancing the FL torque. a, Magnetization change measured by recording the difference of the Hall resistance before and after the pulse as a function of the applied voltage Up and the in-plane external field By . ∆RH is proportional to the fraction of the dot area that has reversed its magnetization, averaged over 200 switching events. The x-component of the external field is fixed to 92 mT. b, Threshold voltage at 50 % switching as a function of By . Inset: schematic of the field direction. For a negative current, By opposes (favors) B F L for By > 0 (By < 0). along the y-direction and has no projection along the easy axis, the effects of this torque are usually neglected in models of the SOT-induced DW dynamics. However, the polar component BθF L ∝ Mz My / sin θ points upward or downward depending on the sign of My , as illustrated by the blue arrows in Fig. 3e. Therefore, the rotation of the magnetization and the nucleation of a reverse domain are favored whenever BθF L and BθDL are parallel to each other, as indicated by the red dots in Fig. 3, and hindered when they are antiparallel. This qualitative argument is supported by harmonic Hall voltage measurements 2 of the FL and DL torques in our samples, which show that B F L and B DL have comparable amplitudes of about 20 mT per 108 A/cm2 , and by both macrospin and micromagnetic simulations that take these torques into account (see Supplementary Information). We note that, in principle, also the z-component of the Oersted field generated by the current flowing in the Pt line can induce a similar top/bottom asymmetry as reported here and assist the nucleation process. However, while Oersted field-assisted switching is of interest for device applications, we find that its effects are minor in the present case, as the closest edge of the Co dot is about 125 nm from the edge of the current line and the Oersted field is significantly smaller compared to the FL torque (see Supplementary Information). Role of the FL torque in promoting the switching efficiency To further investigate the effect of the FL torque on the reversal process, we performed all-electrical pulsed switching experiments on the replica Pt/Co/AlOx dots in the presence of an additional in-plane field By , applied parallel or antiparallel to B F L . In these experiments, the mag7
Figure 5: Micromagnetic simulations of the reversal process. a, Snapshots of the magnetic configuration at different times. The simulations are run for different values of the FL torque relative to the DL torque (see Methods). b, Contrast difference between two consecutive frames, showing the tilt of the DW. The black area represents the expansion of the reversed domain. c, Simulated time trace of the perpendicular magnetization component during switching. netization of the dot is measured by the anomalous Hall effect after the injection of each current pulse. Figure 4a shows the change of the Hall resistance measured after the injection of negative pulses of increasing amplitude for different values of By . The shift of the different curves, exemplified by the voltage threshold at which 50 % of the dot has reversed its magnetization (Fig. 4b), shows that a negative By , which is parallel to B F L and antiparallel to the in-plane component of the Oersted field, promotes switching, whereas a positive By hampers it. These data support the conclusions drawn from the analysis of the nucleation point, namely that the FL torque plays a crucial role in triggering the reversal process and in enhancing the switching efficiency. Dynamic domain wall propagation A striking feature observed in Figure 3 is that the propagating DW front is tilted relative to the current direction, with a tilt angle of about 45◦ that changes in steps of 90◦ depending on the up/down or down/up DW configuration and the sign of the current. According to recent studies, current-induced DW tilting is a telltale signature of the DMI in perpendicular magnetized nanotracks 30,33 . However, the tilt angle in Fig. 3 is opposite to that predicted by micromagnetic models of 8
Pt/Co heterostructures 30,33,39 and observed by MOKE microscopy in Pt/Co/Ni/Co racetracks 43 . More specifically, the angle between the DW normal and the current direction is ≈ −45◦ for a left-handed up-down DW (↑←↓) at positive current (see panel IV in Fig. 3b) rather than ≈ +45◦ as reported in previous studies. We believe that this inconsistency stems from the neglect of the FL torque in the micromagnetic models of current-induced DW motion as well as from the time-resolved nature of our measurements. The tilt angle in the Pt/Co/AlOx dots is in fact analogous to that induced by an external in-plane magnetic field By , which leads to a rotation of the internal DW magnetization away from the x-axis in order to recover the N´eel configuration favored by the DMI 30,33 . Our micromagnetic simulations, which include B F L as well as B DL and the DMI, correctly reproduce the observed dynamic tilt during DW propagation, as shown in Fig. 5. Moreover, the simulations indicate that the FL torque promotes faster DW propagation in the direction indicated by the arrow in Fig. 5b, which coincides with case II reported in Fig. 3 and may also explain the strong anisotropy of the DW velocity recently reported in extended Pt/Co/AlOx layers 15 . We note further that the DW propagation direction is not related to the bias field Bx , the main purpose of which is to break the spin-canting symmetry due to the DMI, whereas the DW velocity increases with Bx (see Supplementary Information). As the tilt angle depends on the B F L /B DL ratio, the opposite DW tilt relative to the Pt/Co/Ni/Co racetracks 43 may be explained by the different SOT amplitudes in this system. A more important difference, however, is that we probe the dynamic structure of the DW during current injection rather than after the current-induced displacement. Starting from a homogeneous magnetization state, we image the fastest DW front sweeping through the sample, which has opposite tilt with respect to the slowest DW front that survives in steady state conditions 43 . Accordingly, we find that the DW front in our measurements is orthogonal to the direction of largest DW velocity recently reported for Pt/Co/AlOx 15 . These findings show that magnetization switching is boosted in the Pt/Co/AlOx dots by the favorable combination of the domain nucleation symmetry and DW propagation direction, which is such that the fastest DW front can sweep unhindered across the full extension of the dot. As an example of a less favourable case, we simulated the effect of a negative B F L (Fig. 5a). Such a field would move the domain nucleation point to the opposite edge of the dot, while the direction of DW propagation along the x-axis would remain unaltered, leading to a much slower reversal dynamics. Partial switching at sub-threshold current amplitude By calculating the time required for the DW front to cover the central region of the dots, we estimate that the DW velocity is of the order of 400 m/s, corresponding to about 100 m/s per 108 A/cm2 of injected current, in agreement with quasi-static measurements of DW displacements 16 . As magnetization reversal is deterministic and achieved by a single DW traversing the 9
Figure 6: Partial switching induced by sub-threshold current pulses. a, Differential images showing the extent of magnetization reversal (in white) for pulses of increasing voltage amplitude. The differential contrast is obtained by averaging all the frames in a time-sequence after positive pulse injection and subtracting the average of all the frames after negative pulse injection. b, Comparison between the fractional reversed area estimated from the images in a, and the all-electrical switching measured by the Hall resistance on a replica dot. The Hall resistance data are averaged over 200 pulse cycles. The different voltage scale for the two measurements is due to the dispersion of the current in the branches of the Hall cross, which is absent in the STXM measurements. entire sample, the switching timescale is expected to be directly proportional to the lateral sample size. This can lead to switching times of less than 200 ps in structures that are smaller than 100 nm. Moreover, we find that pulses that are either shorter or weaker in amplitude compared to the threshold values required to achieve full switching consistently lead to the reversal of a fraction of the dot area. Figure 6a shows the result of a series of switching measurements taken at increasing values of the voltage applied to the current line. Each frame is a differential image showing the average dot area that reversibly switches the magnetization upon applying positive and negative pulses. The reversed dot area increases monotonically with the pulse amplitude, as illustrated in Fig. 6b, and correlates well with the remanent magnetization measured by the anomalous Hall effect on a replica dot. These measurements show that the critical switching current is mostly dependent on the DW mobility and sample dimensions rather than on the initial nucleation barrier. Further, our results agree with the absence of DW inertia reported in Pt/Co layers 44,45 , consistently with the fast damping of magnetic excitations in SOT devices, and show that partial but reliable switching can be obtained also when working below the current amplitude required for full switching. Conclusions Controlling the speed of magnetic switching by electrical currents is one of the main challenges in nonvolatile memory technologies. Our results demonstrate reliable sub-ns magnetization reversal of perpendicularly magnetized Pt/Co dots induced by SOTs over more than 1012 switching cycles. Time-resolved STXM provides unprecedented
insight into the spatial evolution of the magnetization and SOT-induced dynamics during the reversal process, revealing a four-fold asymmetry in the domain nucleation site at the dot edge and in the DW propagation direction, depending on the relative alignment of current and external field. The fast direction of DW motion is diagonal to the current, opposite to the one observed at steady state in racetrack structures. Our findings are complemented by pulsed switching Hall measurements and micromagnetic simulations, which disclose the role of the FL torque in determining the nucleation and DW dynamics in addition to the DL torque and DMI. We anticipate that tuning the amplitude and sign of the FL torque independently of the DL torque, or engineering structures with a significant Oersted field, may lead to improvements in the efficiency of SOT switching. Moreover, as the switching unfolds along a reproducible and deterministic path, the timing and the extent of magnetization reversal can be reliably controlled by the amplitude and duration of the current pulses as well as by the sample dimensions. References 1. A. D. Kent and D. C. Worledge, “A new spin on magnetic memories,” Nature Nanotech., vol. 10, no. 3, pp. 187–191, 2015. 2. K. Garello, I. M. Miron, C. O. Avci, F. Freimuth, Y. Mokrousov, S. Bl¨ ugel, S. Auffret, O. Boulle, G. Gaudin, and P. Gambardella, “Symmetry and magnitude of spin-orbit torques in ferromagnetic heterostructures,” Nature Nanotech., vol. 8, no. 8, pp. 587– 93, 2013. 3. J. Kim, J. Sinha, M. Hayashi, M. Yamanouchi, S. Fukami, T. Suzuki, S. Mitani, and H. Ohno, “Layer thickness dependence of the current-induced effective field vector in Ta—CoFeB—MgO,” Nature Mater., vol. 12, no. 3, pp. 240–5, 2013. 4. J. Sinova, S. O. Valenzuela, J. Wunderlich, C. Back, and T. Jungwirth, “Spin hall effects,” Rev. Mod. Phys., vol. 87, no. 4, p. 1213, 2015. 5. A. Manchon and S. Zhang, “Theory of nonequilibrium intrinsic spin torque in a single nanomagnet,” Phys. Rev. B, vol. 78, p. 212405, 2008. 6. F. Freimuth, S. Bl¨ ugel, and Y. Mokrousov, “Direct and inverse spin-orbit torques,” Phys. Rev. B, vol. 92, no. 6, p. 064415, 2015. 7. L. Wang, R. Wesselink, Y. Liu, Z. Yuan, K. Xia, and P. J. Kelly, “Giant Room Temperature Interface Spin Hall and Inverse Spin Hall Effects,” Phys. Rev. Lett., vol. 116, no. 19, p. 196602, 2016.
8. V. Amin and M. Stiles, “Spin Transport at Interfaces with Spin-Orbit Coupling: Phenomenology,” Phys. Rev. B, vol. 94, no. 10, p. 104420, 2016. 9. I. M. Miron, K. Garello, G. Gaudin, P.-J. Zermatten, M. V. Costache, S. Auffret, S. Bandiera, B. Rodmacq, A. Schuhl, and P. Gambardella, “Perpendicular switching of a single ferromagnetic layer induced by in-plane current injection,” Nature, vol. 476, no. 7359, pp. 189–93, 2011. 10. L. Liu, C.-F. Pai, Y. Li, H. W. Tseng, D. C. Ralph, and R. A. Buhrman, “Spin-torque switching with the giant spin Hall effect of tantalum,” Science, vol. 336, no. 6081, pp. 555–558, 2012. 11. K. Garello, C. O. Avci, I. M. Miron, M. Baumgartner, A. Ghosh, S. Auffret, O. Boulle, G. Gaudin, and P. Gambardella, “Ultrafast magnetization switching by spin-orbit torques,” Appl. Phys. Lett., vol. 105, no. 21, p. 212402, 2014. 12. S. Fukami, T. Anekawa, C. Zhang, and H. Ohno, “A spin–orbit torque switching scheme with collinear magnetic easy axis and current configuration,” Nature Nanotech., 2016. 13. A. Ghosh, K. Garello, C. O. Avci, M. Gabureac, and P. Gambardella, “InterfaceEnhanced Spin-Orbit Torques and Current-Induced Magnetization Switching of Pd/Co/AlOx Layers,” Phys. Rev. Appl., vol. 7, p. 014004, 2017. 14. G. Yu, P. Upadhyaya, K. L. Wong, W. Jiang, J. G. Alzate, J. Tang, P. K. Amiri, and K. L. Wang, “Magnetization switching through spin-Hall-effect-induced chiral domain wall propagation,” Phys. Rev. B, vol. 89, no. 10, p. 104421, 2014. 15. C. Safeer, E. Ju´e, A. Lopez, L. Buda-Prejbeanu, S. Auffret, S. Pizzini, O. Boulle, I. M. Miron, and G. Gaudin, “Spin–orbit torque magnetization switching controlled by geometry,” Nature Nanotech., vol. 11, no. 2, pp. 143–146, 2016. 16. I. M. Miron, T. Moore, H. Szambolics, L. D. Buda-Prejbeanu, S. Auffret, B. Rodmacq, S. Pizzini, J. Vogel, M. Bonfim, A. Schuhl, and G. Gaudin, “Fast current-induced domain-wall motion controlled by the Rashba effect,” Nature Matererials, vol. 10, no. 6, pp. 419–23, 2011. 17. S. Emori, U. Bauer, S.-M. Ahn, E. Martinez, and G. S. D. Beach, “Current-driven dynamics of chiral ferromagnetic domain walls,” Nature Mater., vol. 12, no. 7, pp. 611– 6, 2013. 18. K.-S. Ryu, L. Thomas, S.-H. Yang, and S. Parkin, “Chiral spin torque at magnetic domain walls,” Nature Nanotech., vol. 8, no. 7, pp. 527–33, 2013. 12
19. P. P. J. Haazen, E. Mur`e, J. H. Franken, R. Lavrijsen, H. J. M. Swagten, and B. Koopmans, “Domain wall depinning governed by the spin Hall effect,” Nature Mater., vol. 12, no. 4, pp. 299–303, 2013. 20. M. Cubukcu, O. Boulle, M. Drouard, K. Garello, C. Onur Avci, I. Mihai Miron, J. Langer, B. Ocker, P. Gambardella, and G. Gaudin, “Spin-orbit torque magnetization switching of a three-terminal perpendicular magnetic tunnel junction,” Appl. Phys. Lett., vol. 104, no. 4, p. 042406, 2014. 21. G. Prenat, K. Jabeur, P. Vanhauwaert, G. Di Pendina, F. Oboril, R. Bishnoi, M. Ebrahimi, N. Lamard, O. Boulle, K. Garello, et al., “Ultra-Fast and HighReliability SOT-MRAM: From Cache Replacement to Normally-Off Computing,” IEEE TMSCS, vol. 2, no. 1, pp. 49–60, 2016. 22. T. Devolder, J. Hayakawa, K. Ito, H. Takahashi, S. Ikeda, P. Crozat, N. Zerounian, J.-V. Kim, C. Chappert, and H. Ohno, “Single-shot time-resolved measurements of nanosecond-scale spin-transfer induced switching: Stochastic versus deterministic aspects,” Phys. Rev. Lett., vol. 100, no. 5, p. 057206, 2008. 23. C. Hahn, G. Wolf, B. Kardasz, S. Watts, M. Pinarbasi, and A. D. Kent, “Timeresolved studies of the spin-transfer reversal mechanism in perpendicularly magnetized magnetic tunnel junctions,” Phys. Rev. B, vol. 94, no. 21, p. 214432, 2016. 24. K.-S. Lee, S.-W. Lee, B.-C. Min, and K.-J. Lee, “Threshold current for switching of a perpendicular magnetic layer induced by spin Hall effect,” Appl. Phys. Lett., vol. 102, no. 11, p. 112410, 2013. 25. J. Park, G. E. Rowlands, O. J. Lee, D. C. Ralph, and R. A. Buhrman, “Macrospin modeling of sub-ns pulse switching of perpendicularly magnetized free layer via spinorbit torques for cryogenic memory applications,” Appl. Phys. Lett., vol. 105, no. 10, p. 102404, 2014. 26. C. Zhang, S. Fukami, H. Sato, F. Matsukura, and H. Ohno, “Spin-orbit torque induced magnetization switching in nano-scale Ta/CoFeB/MgO,” Appl. Phys. Lett., vol. 107, no. 1, p. 012401, 2015. 27. S. V. Aradhya, G. E. Rowlands, J. Oh, D. C. Ralph, and R. A. Buhrman, “Nanosecond-Timescale Low Energy Switching of In-Plane Magnetic Tunnel Junctions through Dynamic Oersted-Field-Assisted Spin Hall Effect,” Nano Letters, vol. 16, no. 10, pp. 5987–5992, 2016.
28. R. Lo Conte, A. Hrabec, A. Mihai, T. Schulz, S.-J. Noh, C. Marrows, T. Moore, and M. Kl¨aui, “Spin-orbit torque-driven magnetization switching and thermal effects studied in Ta\ CoFeB\ MgO nanowires,” Appl. Phys. Lett., vol. 105, no. 12, p. 122404, 2014. ´ Ju´e, V. Cros, and A. Fert, “Dynamics of Dzyaloshinskii 29. A. Thiaville, S. Rohart, E. domain walls in ultrathin magnetic films,” Europhys. Lett., vol. 100, no. 5, p. 57002, 2012. 30. O. Boulle, S. Rohart, L. D. Buda-Prejbeanu, E. Ju´e, I. M. Miron, S. Pizzini, J. Vogel, G. Gaudin, and A. Thiaville, “Domain Wall Tilting in the Presence of the Dzyaloshinskii-Moriya Interaction in Out-of-Plane Magnetized Magnetic Nanotracks,” Phys. Rev. Lett., vol. 111, no. 21, p. 217203, 2013. 31. E. Martinez, S. Emori, and G. S. D. Beach, “Current-driven domain wall motion along high perpendicular anisotropy multilayers: The role of the Rashba field, the spin Hall effect, and the Dzyaloshinskii-Moriya interaction,” Appl. Phys. Lett., vol. 103, no. 7, p. 072406, 2013. 32. N. Perez, E. Martinez, L. Torres, S.-H. Woo, S. Emori, and G. S. D. Beach, “Chiral magnetization textures stabilized by the Dzyaloshinskii-Moriya interaction during spin-orbit torque switching,” Appl. Phys. Lett., vol. 104, no. 9, p. 092403, 2014. 33. E. Martinez, S. Emori, N. Perez, L. Torres, and G. S. Beach, “Current-driven dynamics of Dzyaloshinskii domain walls in the presence of in-plane fields: Full micromagnetic and one-dimensional analysis,” J. Appl. Phys., vol. 115, no. 21, p. 213909, 2014. 34. K.-S. Lee, S.-W. Lee, B.-C. Min, and K.-J. Lee, “Thermally activated switching of perpendicular magnet by spin-orbit spin torque,” Appl. Phys. Lett., vol. 104, no. 7, p. 072413, 2014. 35. W. Legrand, R. Ramaswamy, R. Mishra, and H. Yang, “Coherent Subnanosecond Switching of Perpendicular Magnetization by the Fieldlike Spin-Orbit Torque without an External Magnetic Field,” Phys. Rev. Appl., vol. 3, p. 064012, 2015. 36. O. J. Lee, L. Q. Liu, C. F. Pai, Y. Li, H. W. Tseng, P. G. Gowtham, J. P. Park, D. C. Ralph, and R. a. Buhrman, “Central role of domain wall depinning for perpendicular magnetization switching driven by spin torque from the spin Hall effect,” Phys. Rev. B, vol. 89, no. 2, p. 024418, 2014.
37. G. Finocchio, M. Carpentieri, E. Martinez, and B. Azzerboni, “Switching of a single ferromagnetic layer driven by spin Hall effect,” Appl. Phys. Lett., vol. 102, no. 21, p. 212410, 2013. 38. N. Mikuszeit, O. Boulle, I. Miron, K. Garello, P. Gambardella, G. Gaudin, and L. Buda-Prejbeanu, “Spin-orbit torque driven chiral magnetization reversal in ultrathin nanostructures,” Phys. Rev. B, vol. 92, no. 14, p. 144424, 2015. 39. E. Martinez, L. Torres, N. Perez, M. A. Hernandez, V. Raposo, and S. Moretti, “Universal chiral-triggered magnetization switching in confined nanodots,” Sci. Rep., vol. 5, 2015. 40. J. Raabe, G. Tzvetkov, U. Flechsig, M. B¨oge, A. Jaggi, B. Sarafimov, M. G. C. Vernooij, T. Huthwelker, H. Ade, D. Kilcoyne, T. Tyliszczak, R. H. Fink, and C. Quitmann, “PolLux: A new facility for soft x-ray spectromicroscopy at the Swiss Light Source,” Rev. Sci. Instrum., vol. 79, no. 11, 2008. 41. S. Pizzini, J. Vogel, S. Rohart, L. Buda-Prejbeanu, E. Ju´e, O. Boulle, I. M. Miron, C. Safeer, S. Auffret, G. Gaudin, et al., “Chirality-induced asymmetric magnetic nucleation in Pt/Co/AlOx ultrathin microstructures,” Phys. Rev. Lett., vol. 113, no. 4, p. 047203, 2014. 42. M. Belmeguenai, J.-P. Adam, Y. Roussign´e, S. Eimer, T. Devolder, J.-V. Kim, S. M. Cherif, A. Stashkevich, and A. Thiaville, “Interfacial Dzyaloshinskii-Moriya interaction in perpendicularly magnetized Pt/Co/AlOx ultrathin films measured by Brillouin light spectroscopy,” Phys. Rev. B, vol. 91, p. 180405, 2015. 43. K.-S. Ryu, L. Thomas, S.-H. Yang, and S. S. Parkin, “Current Induced Tilting of Domain Walls in High Velocity Motion along Perpendicularly Magnetized MicronSized Co/Ni/Co Racetracks,” Appl. Phys. Express, vol. 5, no. 9, p. 093006, 2012. 44. J. Vogel, M. Bonfim, N. Rougemaille, O. Boulle, I. M. Miron, S. Auffret, B. Rodmacq, G. Gaudin, J. Cezar, F. Sirotti, et al., “Direct observation of massless domain wall dynamics in nanostripes with perpendicular magnetic anisotropy,” Phys. Rev. Lett., vol. 108, no. 24, p. 247202, 2012. 45. T. Taniguchi, K.-J. Kim, T. Tono, T. Moriyama, Y. Nakatani, and T. Ono, “Precise control of magnetic domain wall displacement by a nanosecond current pulse in Co/Ni nanowires,” Appl. Phys. Express, vol. 8, no. 7, p. 073008, 2015. 46. C. O. Avci, K. Garello, M. Gabureac, A. Ghosh, A. Fuhrer, S. F. Alvarado, and P. Gambardella, “Interplay of spin-orbit torque and thermoelectric effects in ferromagnet / normal-metal bilayers,” Phys. Rev. B, vol. 90, p. 224427, 2014. 15
47. M. J. Donahue and D. G. Porter, OOMMF User’s Guide, Version 1.0. Interagency Report NISTIR 6376, National Institute of Standards and Technology, Gaithersburg, MD (Sept 1999). 48. S. Rohart and A. Thiaville, “Skyrmion confinement in ultrathin film nanostructures in the presence of Dzyaloshinskii-Moriya interaction,” Phys. Rev. B, vol. 88, p. 184422, 2013.
Acknowledgments This work was funded by the Swiss National Science Foundation (Grant No. 200021153404). We acknowledge fruitful discussions with J. St¨ohr and L. Buda-Prejbeanu.
Author contributions M.B., K.G., and P.G. planned the experiments and analyzed the data. M.B., M.G., and J.F. fabricated the samples. M.B., K.G., J.M., C.O.A., E.G., C.M., C.S., Y.A., S.F., S.W., and J.R. implemented the current pump / x-ray probe scheme and performed the STXM experiments. M.B. carried out the electrical measurements and the micromagnetic simulations. M.B. and P.G. wrote the manuscript. All authors discussed the data and commented on the manuscript.
Additional information Correspondence and requests for materials should be addressed to M.B. (manuel.bau[email protected]
) and P.G. ([email protected]
Methods Sample fabrication The samples were fabricated on 200 nm thick Si3 N4 membranes supported by a rigid Si frame. The Pt(5 nm)/Co(1 nm)/Al(1.6 nm) layer was deposited by dc magnetron sputtering at a base pressure of 4 · 10−8 mTorr and the Al cap layer was subsequently oxidized in an O2 atmosphere of 13 mTorr for 35 s and a power of 36 W. Circular Co dots with 500 nm diameter and 750 nm wide Pt current lines were patterned by electron beam lithography followed by an ion milling process optimized to stop at the Pt/Co interface and at the Si3 N4 /Pt interface, respectively. Au contacts for current injection were fabricated in the proximity of the Co dots using UV-photo lithography and lift-off. Finally, a 100 nm thick Al layer was deposited by sputtering on the backside of 16
the membrane in order to efficiently dissipate the heat originating from current-induced Joule heating. Scanning transmission x-ray microscopy The magnetization of the dots was imaged by time-resolved scanning transmission x-ray microscopy at the PolLux beamline of the Swiss Light Source 40 using a current pump / x-ray probe scheme. This method uses a Fresnel zone plate to focus a monochromatic x-ray beam onto the sample, which is scanned through the x-ray focus while an avalanche photodiode collects the transmitted photon intensity. Typical dot images are obtained by recording the x-ray intensity over a twodimensional 64 × 64 pixel array with about 25 nm lateral resolution. The pump current consists of a bipolar pulse sequence that has a total length of 102.1 ns. Each unit sequence includes one positive and one negative pulse spaced by 50 ns, the length and amplitude of which can be tuned independently from each other. The magnetization state is probed by exploiting the XMCD contrast at the Co L3 absorption edge (E = 779 eV) using left circularly polarized light at normal incidence. The probe x-ray beam has a 70 ps wide bunch structure with a repetition rate of 500 MHz. The magnetization is thus sampled every 2 ns results in a time resolution of 100 ps after the injection of 20 successive unitsequences by routing the intensity of each probing event to a counting register. The current pulse sequences run continuously during the measurements, synchronized to the x-ray pulses, and are monitored by means of a -20 dB pick-off tee connected to an oscilloscope. The amplitude of the pulses is reported in voltage units, with Up = 1 V corresponding to a current density jp = 8.4 · 107 A/cm2 in the Pt line. Electrical measurements Replicas of the dots were fabricated on Si3 N4 membranes with the Pt underlayer patterned in the shape of a Hall cross (see Supplementary Fig. 1). These samples were deposited and processed together with those used for the xray measurements. We performed all-electrical pulsed switching measurements using the anomalous Hall resistance to detect the magnetization state after current injection 1 . The Hall measurements are averaged over 200 set pulses with length 2 ns, each followed by a stronger reset pulse to ensure that the magnetization reverts to a homogeneous state before injection of the next set pulse. The Harmonic Hall voltage measurements of the SOTs 2,3 were performed on 5 µm wide Pt/Co/AlOx Hall bars, which were also deposited and processed simultaneously with the dots. These measurements, corrected for a small contribution due to the Nernst effect 4 , give B DL = 18 mT and B F L = B0F L + B2F L sin2 θ, where θ is the polar angle of the magnetization relative to the z-axis, B0F L = 10.2 mT, and B2F L = 18 mT for a current density of 108 A/cm2 (see Supplementary Information).
Micromagnetic simulations Micromagnetic simulations based on the integration of the Landau-Lifshitz Gilbert equation were performed using the object oriented micromagnetic framework (OOMMF) code 47 , including the DMI extension module 48 as well as the DL and FL SOTs. All simulations of the 500 nm wide and 1 nm thick Co dot were carried out using a cell size of 4 nm × 4 nm × 1 nm with the following material parameters: saturation magnetization Ms = 900 kA/m, exchange coupling constant Aex = 10−11 A/m, uniaxial anisotropy energy Ku = 657 kJ/m3 , DMI D = 1.2 mJ/m3 , and damping constant α = 0.5. The magnitude of the DL and FL torques corresponds to the values measured by the harmonic Hall voltage method; the in-plane bias field is set to Bx = 93 mT. The simulated current pulse has an amplitude of jp = 4.5 · 108 A/cm2 and a duration of τp = 2 ns. All simulations were carried out at zero temperature.
SUPPLEMENTARY INFORMATION Time- and spatially-resolved magnetization dynamics driven by spin-orbit torques M. Baumgartner,1 K. Garello,1,2 J. Mendil,1 C. O. Avci,1 E. Grimaldi,1 C. Murer,1 J. Feng,1 M. Gabureac,1 C. Stamm,1 Y. Acremann,3 S. Finizio,4 S. Wintz,4 J. Raabe,4 P. Gambardella1 1 Department
of Materials, ETH Z¨ urich, 8093 Z¨ urich, Switzerland,
2 IMEC, 3 Laboratory
Kapeldreef 75, 3001 Leuven, Belgium,
for Solid State Physics, ETH Z¨ urich, 8093 Z¨ urich, Switzerland,
Scherrer Institute, 5232 Villigen PSI, Switzerland
Contents SI1 Magnetic characterization and all-electrical pulsed switching measurements
SI2 Harmonic Hall voltage measurements of the spin-orbit torques
SI3 Dependence of the switching speed on the external field Bx
SI4 Macrospin model of magnetization reversal at different edge positions
SI5 Effect of the Oersted field
SI6 Switching of defective dots
SI7 Comparison between filtered and raw data
Magnetic characterization and all-electrical pulsed switching measurements
Figure S1a shows an atomic force microscope image of a 500 nm wide Co dot on top of a Pt Hall cross deposited on a 200 nm thick Si3 N4 membrane. The Co dot is 1 nm thick, capped by 2 nm of oxidized Al, and the Pt line is 5 nm thick. This type of samples are replicas of those employed for the STXM measurements, which we used to characterize the magnetic properties and to perform all-electrical pulsed switching experiments by probing the anomalous Hall effect S1 . Figure S1b shows the Hall resistance RH = RAHE cos θ = RAHE Mz measured as a function of the external field Bext applied out-of-plane (θB = 0◦ ) and nearly in-plane (θB = 84◦ ). Here, θ and θB are the polar angles of the magnetization and applied field, respectively, and RAHE is the anomalous Hall coefficient. The square loop measured at θB = 0◦ shows that the dots have strong perpendicular magnetic anisotropy, with an effective anisotropy field given by BK = Bext (sin θB / sin θ − cos θB / cos θ) ≈ 660 mT. Figure S1c shows pulsed switching measurements as a function of the pulse voltage amplitude Up (1 V corresponds to jp = 8.4 · 108 A/cm2 in the Pt line) for different pulse
Figure S1: Magnetic characterization and all-electrical pulsed switching measurements. a, Atomic force microscopy image showing a 500 nm Co dot on a 750 nm wide Pt Hall cross grown on a Si3 N4 membrane. b, RH measured as a function of external field applied out-of-plane (left panel, θB = 0◦ ) and nearly in-plane (right panel, θB = 84◦ ). c, Pulsed magnetization switching measurements as a function of pulse length (left panel) and in-plane bias field (right panel). In both cases the bias field is applied at an angle θB = 89◦ along the current line. 2
widths τp and external fields applied at an angle θB = 89◦ , almost parallel to the current line. Each point represents the difference of the Hall resistance measured after and before the pulse averaged over 200 switching attempts starting from a fully saturated magnetization state. We observe reliable switching at pulse voltages and widths comparable to those used for the STXM measurements, the main difference being that the Up values in the Hall measurements are about 20 % larger compared to the x-ray measurements due to the dispersion of the current in the Hall cross. In agreement with previous studies S1 , we find that the threshold pulse amplitude to achieve switching decreases with increasing pulse width and bias field. SI2
Harmonic Hall voltage measurements of the spin-orbit torques
In order to determine the SOTs and the effective perpendicular anisotropy field in our structures, we performed z adiabatic harmonic Hall voltage measurements S2,S3 using an ac current of frequency ω = 2π · 10 Hz and a eϕ M current density of j = 107 A/cm2 . The sample is a θ eθ θΒ 5 µm wide Hall bar which has been deposited on Si3 N4 Bext y ϕ at the same time as the Co dots used for the timej x resolved switching experiments described in the main text. The injection of the ac current into the Pt/Co Figure S2: Coordinate scheme. bilayers generates a Hall voltage perpendicular to the current direction, which depends on the orientation of the magnetization due to the anomalous and planar Hall effects. The Hall resistance ω 2ω RH = VH /I = RH + RH includes a first and a second harmonic component. The first harmonic component, shown in the top panels of Fig. S3, is equivalent to the dc Hall resistance, which depends on the equilibrium position of the magnetization as ω RH = RAHE cos θ + RP HE sin2 θ sin(2ϕ),
where RP HE is the planar Hall coefficient and ϕ the azimuthal angle describing the inplane orientation of the magnetization relative to the x-axis (see Fig. S2). The second harmonic signal, which is proportional to the current, depends on the SOT-induced reorientation of the magnetization about the equilibrium position as well as on magnetothermal 2ω effects scaling with I 2 . The general form of RH is given by S2,S4 2ω RH = [RAHE − 2RP HE cos θ sin(2ϕ)]
BθI 2 cos(2ϕ) I d cos θ 2ω +RP HE sin2 θ B +R∇T , dBext sin(θB − θ) Bext sin θB ϕ (S2)
where BθI and BϕI are the polar and azimuthal components of the total current-induced ω field BI = BDL + BF L + BOe . By performing three independent measurements of RH 2ω and RH at different angles (for instance at ϕB = 0 ◦ , 45 ◦ , 90 ◦ , as shown in Fig. S3) with a fixed θB , these components can be directly linked to the SOTs expressed in spherical coordinates: BF L = BθF L cos θ sin ϕeθ + BϕF L cos ϕeϕ , (S3) BDL = BθDL cos ϕeθ − BϕDL cos θ sin ϕeϕ ,
where eϕ and eθ are the azimuthal and polar unit vectors. The last term in Eq. (S2) is the magnetothermal Hall resistance, which is mainly due to the anomalous Nernst effect induced by Joule heating. This term must be taken into account for accurate SOT 2ω quantification. The second harmonic components due to R∇T and the current-induced 2ω fields are separated by analyzing the dependence of RH on Bext during a field scan with ◦ ◦ θB = 90 and ϕB = 45 . As the magnetization saturates in the sample plane at high 2ω 2ω 2ω fields, the susceptibility to the SOT decreases and RH → R∇T . Plotting RH as a function 2ω of 1/(Bext − BK ) allows us to deduce R∇T from the intercept of the coordinate axis S4 . 2ω leads to a reduction of the SOTs of about 20 % In the present case, accounting for R∇T 2ω . (15 %) for the FL (DL) torque relative to the values derived from the as-measured RH F L,Oe Following this procedure we find that B DL = 18 mT, and B F L = B0 + B2F L sin2 θ,
Figure S3: Harmonic Hall voltage measurements of the SOTs. Upper row: First harmonic Hall resistance signals obtained for ϕB = 0 ◦ , ϕB = 45 ◦ and ϕB = 90 ◦ at constant θB = 86 ◦ . Lower row: Corresponding second harmonic signal.
where B0F L,Oe = 10.2 mT and B2F L = 18 mT for a current density of 108 A/cm2 . The Oersted field contribution is evaluated in Sect. SI5. SI3
Dependence of the switching speed on the external field Bx
Figure S4a shows the XMCD time traces of a Co dot during the injection of 2 ns long current pulses of amplitudes Up =-3.35 V and 3.42 V at different values of the applied field Bx . In the following, we will limit the discussion to negative fields but emphasize that the same arguments are consistent with positive bias fields. We find that Bx has an influence on the reversal speed, namely that switching occurs faster at high field values. This is shown in Fig. S4b where the average slope of the XMCD time traces during the reversal is plotted against Bx . With increasing Bx , Mz decreases while |Mx | increases on one side of the dot, which favours magnetization reversal. Our findings are supported by micromagnetic simulations (see Methods Section) in
Figure S4: Effect of the external in-plane field on the switching speed. a, Measured XMCD time traces as a function of in-plane field Bx . b, Average slope of the rising and falling edges during the reversal plotted as function of Bx . c, Simulated time traces of Mz as a function of Bx . The slow dynamics after the current pulse is z due the DW reorientation after incomplete magnetization reversal. d, Reversal rate dM dt evaluated for the traces shown in c during the current pulse. 5
which we analyze the influence of Bx on the reversal speed. Figure S4c shows the simulated time traces of Mz following the injection of a current pulse of amplitude jp = 4.5·108 A/cm2 for different values of Bx . The simulations show that there is a threshold bias field 63 mT < Bx < 73 mT below which reversal does not take place. Above this field, the DW velocity increases with Bx as the magnetization tilts more towards the sample plane and the energy barrier for DW propagation reduces, in agreement with the experiment. We further note that the experimental threshold field can be significantly lower compared to the simulations owing to Joule heating, which assists the nucleation of reversed domains. SI4
Macrospin model of magnetization reversal at different edge positions
We provide a simplified and intuitive model of the edge nucleation by simulating the reversal process of four non-interacting single spins located at positions (1) - (4) around the Co dot, as illustrated in Fig. S5a. The DMI is included as an effective field by considering the DMI-energy EDM I = D · (Mi × S) , (S5) where Mi is the magnetization vector of the spin at position (i), S represents a fictitious central spin of fixed orientation and D is the DMI-coupling vector. D lies in the sample plane and is perpendicular to the vector connecting the spins Mi and S. It can thus be parametrized by an angle ϕi as D = D(sin ϕi , − cos ϕi , 0). We then make use of the
Figure S5: Macrospin model of edge magnetization reversal. a, Schematic representation of four non-interacting spins located at distinct positions around the dot. The DMI is taken into account as an effective in-plane field, the sign of which depends on the orientation of the fictitious central spin. b, z-component of the four macrospins during the application of a current pulse for B F L > 0 (upper panel, corresponding to the experimental situation) and B F L < 0 (lower panel). 6
general relation BDM I = −∇M EDM I to express the DMI-energy as an effective field
cos ϕi = sgn (Sz ) 2D sin ϕi . 0
Finally, we perform a time-integral of the Landau-Lifshitz Gilbert equation to separately model the evolution of the magnetization at points (1) - (4) under the action of BDM I,i , Bx = 100 mT, effective anisotropy field BK = 657 mT, and the DL and FL torques measured in Section SI2. We choose the DMI-coupling strength D such that it induces a spin canting at the sample edge similar to that reported in Ref. S5 . The canting angle at positions (1) and (2) under a positive bias field of Bx = 100 mT is ≈ 18 ◦ for D = 60 mT, whereas it is ≈ 8 ◦ at positions (3) and (4). For brevity, we limit the discussion to Bx > 0 and positive current pulses, as indicated in Fig. S5a. We consider first the case Sz > 0, which represents the dot in the up-state. For a given current, the simulated time traces of the magnetization at positions (1) - (4), reported in Fig. S5b, show that only the spin located at position (1) reverses, whereas, by inverting the sign of B F L and keeping B DL constant, only the spin at position (2) reverses. This behavior is in agreement with the nucleation point observed experimentally (Fig. 3b (II)). Inverting the sign of the central spin, such that Sz < 0, changes the direction of the effective DMI-field and makes position (3) equivalent to position (1) in the former case (Sz > 0). The effect of the FL torque at different positions can be simply rationalized by considering the θ-component of the field B F L : 0 cos θ cos ϕi = BF L · eθ = B F L · cos θ sin ϕi = B F L cos θ sin ϕi , 0 − sin θ
where we see that BθF L depends on ϕi and points towards the xy-plane at position (1) and in the opposite direction at position (2), thus favoring the reversal of spin (1) relative to (2). SI5
Effect of the Oersted field
The current flowing in the Pt line produces an Oersted field with y- and z-components given by S6
ByOe = −
I Uy+ − Dy+ + Uy− − Dy− ·10−3 , wd
BzOe = −
I Uz+ − Dz+ − Uz− + Dz− ·10−3 , wd (S8)
Figure S6: Influence of the Oersted field on magnetization reversal. a, Calculated Oersted field according to Eq. (S8) at a height of 0.5 nm above the Pt line for a positive current pulse of amplitude 1 · 108 A/cm2 . b, Illustration of the nucleation process supported by the z-component of the Oersted field at positive and c, negative current. d, θ-component of B F L and B Oe as a function of θ during a positive current pulse of amplitude 1 · 108 A/cm2 for a spin located at the position (1) and e, (2) of the dot (see diagram in Fig. S5). f, Simulated time traces for different combinations of B Oe , B F L and B DL . g Corresponding snapshots during the magnetization reversal. 8
where I is the current, w is the width of the Pt line and d its thickness, respectively. The coefficients are defined as follows: w/2 ± y ± + (w/2 ± y) ln (w/2 ± y)2 + (z + d)2 , (S9) Uy = 2(z + d) arctan z+d
w/2 ± y = 2z arctan + (w/2 ± y) ln (w/2 ± y)2 + z 2 , z z+d ± Uz = 2(w/2 ± y) arctan + (z + d) ln (w/2 ± y)2 + (z + d)2 , w/2 ± y z ± Dz = 2(w/2 ± y) arctan + z ln (w/2 ± y)2 + z 2 , w/2 ± y Dy±
(S10) (S11) (S12)
with z being the height above the surface of the Pt line. Figure S6a shows the Oersted field calculated according to Eq. S8-S12 for a current density of 1 · 108 A/cm2 flowing through the Pt layer, at z = 0.5 nm above the Pt surface. The y-component ByOe = −3 mT is approximately constant over the dot surface and directed against B F L . The largest z-component is found at the two extrema of the dots closest to the edge of the Pt line, where |BzOe | = 1.6 mT. The sign of BzOe is opposite on opposite sides of the dot, such that this field can also induce a top/bottom edge asymmetry, supporting the nucleation process induced by B F L , as shown in Figs. S6b and c. To analyze the role played by the Oersted field and FL torque in the nucleation, we plot in Fig. S6d the θ-components of B F L and B Oe as a function of θ. The fields are evaluated at position (1) in Fig. S5, where the magnetization is tilted by the DMI and external field along ϕ = 45◦ . At this position, the total Bθ is positive for all θ, parallel to eθ (Fig. S2), and thus favours the rotation of the magnetization from up to down. However, without B F L magnetization reversal would not be favoured at this position since BθOe is negative over a large range of θ. The opposite argumentation is valid for the magnetization at position (2) in Fig. S5a, where the reversal is favoured by B Oe and hindered by B F L (Fig. S6e). As (1) corresponds to the experimentally observed nucleation, we conclude that B F L is the main cause of the nucleation asymmetry. It is important to note that ByOe is approximately constant over the dot area whereas BzOe increases rapidly near the Pt line edge. This implies that magnetization nucleation will be eventually also assisted by the Oersted field for Co dots with a diameter comparable to the Pt line width. To demonstrate the effect of B Oe on the switching process, we performed a series of micromagnetic simulations with i) B Oe 6= 0 and B F L 6= 0, ii) B Oe = 0 and B F L 6= 0, iii) B Oe 6= 0 and B F L = 0 and iv) B Oe = 0 and B F L = 0, the results of which are reported in Figs. S6f and g. Without B F L the switching efficiency is strongly reduced, whereas the addition 9
Figure S7: Switching in the presence of defects. Images taken at intervals of 100 ps during the injection of 2 ns long current pulses. DW nucleation is observed at different sites. The point at which the reversed domain front collapses (orange dot) is off-centred, in agreement with the preferential DW propagation direction discussed in the main text (green arrows). of B Oe to B F L has only a small influence on the reversal mechanism for the given device geometry. The simulations also show how the nucleation point moves up along the edge for B F L = 0. SI6
Switching of defective dots
All of the measured dots show reproducible switching behavior rather than thermallyinduced stochastic reversal, which would result in uniform STXM contrast during the reversal process. However, approximately 50% of the dots showed defect-promoted switching, likely due to inhomogeneities occurred during the patterning process. Such samples are distinguished by the ones presented in the main text by the fact that nucleation always starts from a given point or region rather than alternating between the four dot quadrants. Figure S7 shows a case of defect-promoted switching in which domain nucleation starts at several points around the Co dot edge. Due to the stroboscopic nature of our measurements, we cannot tell whether the nucleation starts simultaneously at different locations or is randomly distributed over the dot edge. However, we do observe that once a domain has nucleated, the favoured DW propagation direction remains the same (green arrows in Figure S7) and is comparable to the switching behaviour reported in Fig. 3 of the main text. The point at which the reversed domain front collapses (orange dot) is therefore off-centred. Importantly, we find that in all cases the reversal process is robust with respect to the presence of defects, which makes SOT-induced magnetization switching very versatile for applications.
Comparison between filtered and raw data
Given the very low photon count rate at the detector position and the relatively low x-ray absorption contrast corresponding to the 1 nm thick Co layer, the acquisition time of a single sequence of images with 100 ps resolution requires several hours of integration. In order to enhance the magnetic contrast, the intensity of each frame in Fig. 3 of the main text and Fig. S7 has been normalized to the non-magnetic background. Moreover, to improve the signal-to-noise ratio, the intensity of each pixel has been low-pass filtered along the time axis. We have checked that the filtering process does not introduce a significant distortion of the data. For completeness, we compare below the raw and filtered images side-by-side in Figs. S8 and S9. Multi-frame movies constructed from the same series of images are included as separate files in the Supplementary Material.
Figure S8: Comparison of the raw and filtered data shown in Fig. 3. a, Raw and b, low-pass filtered images.
Figure S9: Comparison of the raw and filtered data shown in Fig. S7. a, Raw and b, low-pass filtered images.
References 1. K. Garello, C. O. Avci, I. M. Miron, M. Baumgartner, A. Ghosh, S. Auffret, O. Boulle, G. Gaudin, and P. Gambardella, “Ultrafast magnetization switching by spin-orbit torques,” Appl. Phys. Lett., vol. 105, no. 21, p. 212402, 2014. 2. K. Garello, I. M. Miron, C. O. Avci, F. Freimuth, Y. Mokrousov, S. Bl¨ ugel, S. Auffret, O. Boulle, G. Gaudin, and P. Gambardella, “Symmetry and magnitude of spin-orbit torques in ferromagnetic heterostructures,” Nature Nanotech., vol. 8, no. 8, pp. 587– 93, 2013. 3. J. Kim, J. Sinha, M. Hayashi, M. Yamanouchi, S. Fukami, T. Suzuki, S. Mitani, and H. Ohno, “Layer thickness dependence of the current-induced effective field vector in Ta—CoFeB—MgO,” Nature Mater., vol. 12, no. 3, pp. 240–5, 2013. 4. C. O. Avci, K. Garello, M. Gabureac, A. Ghosh, A. Fuhrer, S. F. Alvarado, and P. Gambardella, “Interplay of spin-orbit torque and thermoelectric effects in ferromagnet / normal-metal bilayers,” Phys. Rev. B, vol. 90, p. 224427, 2014. 5. N. Mikuszeit, O. Boulle, I. Miron, K. Garello, P. Gambardella, G. Gaudin, and L. Buda-Prejbeanu, “Spin-orbit torque driven chiral magnetization reversal in ultrathin nanostructures,” Phys. Rev. B, vol. 92, no. 14, p. 144424, 2015. 6. M. Hayashi, J. Kim, M. Yamanouchi, and H. Ohno, “Quantitative characterization of the spin-orbit torque using harmonic Hall voltage measurements,” Phys. Rev. B, vol. 89, no. 14, p. 144425, 2014.